Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites

 Valentine Thornton
 7 months ago
 Views:
Transcription
1 Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A. Aboutorabi 1 Summary The compliance equation is used to calculate the energy release rate for angle ply laminated double cantilever composite beam specimen. Instead of the traditional approach of a beam on an elastic foundation, a second order shear thickness deformation beam theory (SSTDBT) has been considered. keywords: Double Cantilever Beam, Energy Release Rate, Fracture Energy Introduction Fiberreinforced composite materials are widely used in all kinds of engineering structures owing to their high strengths and low densities. Laminated composite structures are made up of layers of orthotropic materials that are bonded together. The layers may be of different materials, or of the same orthotropic material, with the principal material directions of each layer oriented at different angles to the reference axes. By altering material or orientation, or both, of each layer, a structural designer can tailor the strength and other properties of a laminate to the requirements of a given application. Because of the low stiffness in the transverse direction, when outofplane loading exists, separation between plies occurs, i.e. delamination. The presence and growth of delamination under static or fatigue loadings will lead to safety problems by reduction of structural stiffness or initiating catastrophic fracture [1 4]. Hence in any engineering design of laminated composite structures, the delamination mode of failure should be taken into account [5,6]. Usually the delamination modes in composite laminates contain Mode I (opening), Mode II (in plane shearing) and Mode III (out of plane tearing) fractures. Therefore, it is important to characterize these fracture modes to prevent delamination damage. The overwhelming literature on delamination is mainly related to unidirectional composites. A feature that complicates the analysis of delamination growth in angle ply laminates is that delamination exists between angleplies (e.g.±θ). In an optimum laminate design, the objective will be to minimize the crack driving force and/or the crackinduced interfacial principal tensile stress in the angleply laminate under transverse shear loading. This problem is cast as a single or multicriterion optimization problem. The design variables are the ply angle θ and the relative ply thicknesses of the sublaminates. It is recognized that a delamination between angleplies has the feature of a crack between dissimilar anisotropic materials which substantially complicates the fracture mechanics analysis. 1 Faculty of Engineering, Kingston University, UK. Corresponding author:
2 62 Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 The double cantilever beam (DCB) test [7] is the most widely used method for determining the Mode I toughness of composite materials. The test specimen, the applied load, P, to the two arms and the corresponding load line displacement, δ, are schematically illustrated in Fig. 1. A model based on an EulerBernoulli beam on an elastic Winkler foundation for analysing the DCB specimen was originally developed by Kanninen [8,9] for isotropic materials and by Williams [10] for transversely isotropic materials. This model is extended to angleply laminates by Ozdil and Carlsson [11]. The beam displacements derived from this model are used to calculate the compliance and strain energy release rate of the DCB specimen. Recently, Hamed et al. [12], introduced an improved analytical model for delamination in composite beams under general edge loading which also takes into account the shearthickness deformation. In the present study, Hamed model together with the compliance equation has been used to develop a method of determining the Mode I interlaminar fracture toughness in thick angle ply laminated composites. Figure 1: Angle ply DCB specimen divided into three regions Theoretical Analysis Consider the DCB specimen in Fig. 1 made of an angle ply laminate and divided into three regions I, II and III. Assuming a second order shear thickness deformation beam theory (SSTDBT), the displacement field is u 1 (x,y,z)=u(x)+zψ x (x)+z 2 η x (x), u 2 (x,y,z)=0, (1) u 3 (x,y,z)=w(x)+zψ z (x), in all three regions, where u 1, u 2 and u 3 are the displacement components of a point in the x, y and z directions, respectively. Note that the superscripts I, II and III will be given to all of the displacement components to distinct them for the regions I, II and III. SubstitutingEq. 1 into the straindisplacement relations of elasticity we obtain ε x = ε1 0 +zκ0 1 +z 2 κ1, 1 ε y = 0, ε z = ε3, 0 γ yz = 0, γ xz = ε5 0 +zκ5 0, γ xy = 0 (2)
3 Calculation of Energy Release Rate 63 where ε 0 1 = u, κ 1 0 = ψ x, κ 1 1 = η x, ε 0 3 = ψ z, ε 0 5 = ψ x +w, κ 0 5 = 2η x +ψ z (3) and a prime denotes differentiation with respect to x. Since we are developing a beam theory, a state of plane stress is presented and therefore σ y = σ yz = 0. (4) Next by imposing Eq. 4 on three dimensional Hooke s law of elasticity, the plane stress constitutive law for the kth layer of each region is σ x σ z σ xy (k) C 11 C 13 C 16 = C 13 C 33 C 36 C 16 C 36 C 66 (k) ε x ε z γ xy (k), σ (k) xz = C (k) 55 γ (k) xz, (5) where C ij = C ij C i2c j2 i, j = 1,3,6 and C 55 = C 55 C (6) C 22 C 44 In Eq. 6, C ij denote offaxis stiffness coefficients of the kth layer [13]. Using the principle of minimum total potential energy, and considering the displacement field in Eq. 1, the equilibrium equations together with the boundary conditions (B.C. s) at boundaries and continuity conditions (C.C. s) and the equilibrium conditions (E.C. s) at the intersection of three regions will be obtained. Further by substituting the laminate constitutive relations into the equilibrium equations, the governingequilibriumequationsintermsof displacement componentsfor thethree regions will be found as A 11 u A 13 ψ z B 11 ψ x D 11 η x = 0, B 11 u B 13 ψ z D 11ψ x E 11η x +A 55(ψ x +w )+B 55 (2η x +ψ z )=0, D 11 u D 13 ψ z E 11 ψ x F 11 η x +2B 55 (ψ x +w )+2D 55 (2η x +ψ z)=0, A 55 (ψ x +w ) B 55 (2η x +ψ z )=0, A 13 u +A 33 ψ z +B 13 ψ x +D 13 η x B 55 (ψ x +w ) D 55 (2η x +ψ z )=0, (7) where A ij, B ij, D ij, E ij and F ij are laminate stiffness coefficients [12]. Giving the superscripts I, II and III to all of the displacement components and also the stiffness coefficients in Eq. 7, a system of ordinary differential equations (ODE) of order 30 will be resulted. This system of ODEs together with the B.C. s, C.C. s and E.C. s can be solved and all displacement components for thethree regions can be obtained.
4 64 Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Hamed [12] calculated the energy release rate using the Jintegral. Here the classical IrwinKies expressions [14] will be used to obtain the strain energy release rate (SERR) from the beam theory solution, i.e., G = P2 δc 2b δa. (8) where in Eq. 8, P is the load, b is the specimen width, a is the crack length and C the compliance is defined as C = δ P, (9) To obtain the G, we must first express C in terms of the crack length a. FromFig. 1, it is obvious that δ = u I 3 u II x = a 3 (10) x = a z = 0 z = 0 Because of complicated computations, however, the problem cannot be solved explicitly in terms of a. Therefore the DCB problem has been solved for a range of crack length and then a leastsquare regression was fitted to obtain C as a function of crack length, a C(a)=C 3 a 3 +C 2 a 2 +C 1 a +C 0 (11) The above equation can be differentiated with respect to crack length a and G is calculated from Eq. 8. Numerical Examples and Discussions Glass/polyester DCB specimens consisting of antisymmetric angle ply laminates of the form [±30 ] 5 and [±45 ] 5 was chosen as those in [11] where h=7.3 mm, b=20 mm, a=35 mm and l= mm. AlsoE 1 = 34.7GPa, E 2 = 8.5GPa, ν 12 = ν 13 = 0.27, ν 23 = 0.5, G 12 = G 13 = 4.34GPa, G 23 = 2.83GPa. Furtherfor θ = 45, E 3 = 9.85GPa and for θ = 30, E 3 = 9.37GPa. Considering these properties, the corresponding C i are presented in Table 1. Table 1: Polynomial coefficients of compliance in Eq. 11. Lay C 0 C 1 C 2 C 3 up [±30 ] e [±45 ] e Fig. 2a compares SERR obtained from the compliance equation with those obtained from JIntegral [12] for two antisymmetric angle ply laminates of θ = 30 and θ = 45,and for various values of crack length at constant applied load of P=40 N. The results are in good agreement with each other. In similar crack lengths,
5 Calculation of Energy Release Rate G [J/m 2 ] G [J/m 2 ] θ = 30 ο Compliance Equation θ = 45 ο Compliance Equation θ = 30 ο J Integral θ = 45 ο J Integral 50 0 q = 30 o  Compliance Equation q = 45 o  Compliance Equation q = 30 o  J Integral q = 45 o  J Integral (a) Figure 2: Comparison of pure mode I strain energy release rate, G, obtained from JIntegral and compliance equation for [±θ] 5 specimens versus (a) Crack length at constant applied load of P=40 N, (b) Applied load P at constant crack length of a=40 mm. (b) P [N] = = 45 Compliance [ m/n] SSTDBT Experiment Compliance [ m/n] SSTDBT Experiment Figure 3: Comparison of Calculated and measured Compliance = 30 = 45 G c [J/m 2 ] SSTDBT EFM G c [J/m 2 ] 200 SSTDBT EFM (a) Figure 4: Comparison of pure mode I fracture energy, G c, obtained from elastic foundation model, EFM [11] and SSTDBT using compliance equation for [±θ] 5 specimens (a) θ = 30 (b) θ = 45. SERR for θ = 45 are greater than when θ = 30. In Fig. 2b, SERR are plotted versus applied load for twoangle plylayups at constantcrack length ofa=40 mm. (b)
6 66 Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Similar to Fig. 2a, the results obtained from compliance equation are in accordance with the results from JIntegral. In Figs. 3 the calculated compliances from SSTDBT theory are compared with the experimental results obtained by Ozdil and Carlsson [11]. It is observed that when θ = 30, SSTDBT underestimates the compliance value but for θ = 45 the results are very close. In Figs. 4 pure mode I fracture energy, G c, obtained from elastic foundation model, EFM [11] and SSTDBT using compliance equation for [±θ] 5 specimens at two angleplies of θ = 30 and θ = 45 are compared. It is shown and verified that the second order shear thickness deformation beam theory (SSTDBT) together with compliance equation accurately estimates the mode I fracture toughness and strain energy release rate for any angleply laminates. The method is robust and general and other mode of fracture can be modelled using this method. References 1. Nicholls DJ, Gallagher JP. Determination of GI C in angleply composites using a cantilever beam test method. J. Reinf. Plast. Compos. 1983;2: Chai H. The characterization of mode I delamination failure in nonwoven, multidirectional laminates. Composites 1984;15: Laksimi A, Benzeggagh ML, Jing G, Hecini M, Roelandt JM. Mode I interlaminar fracture of symmetrical crossply composites. Compos. Sci. Technol. 1991;41: Robinson P, Song DQ. A modified DCB specimen for modei testing of multidirectional laminates. J. Compos. Mater. 1992;26: Johnson WS, editor. Delamination and debonding of materials, ASTM STP 876, Philadelphia, PA, Prel VJ, Davies P, Benzeggagh ML, de Charentenay FX. Mode I and Mode II delamination of thermosetting and thermoplastic composites. ASTM STP 1012, Philadelphia, PA, 1989, pp ASTM Test Method D a Mode I Interlaminar Fracture Toughness of Unidirectional Continuous Fiber Reinforced Composite Materials, Annual Book of ASTM Standards, Vol 15.03, American Society for Testing and Materials, West Conshohocken, PA. 8. Kanninen MF. An augmented double cantilever beam model for studying crack propagation and arrest. Int J Fracture 1973; 9(1): Kanninen MF. A dynamic analysis of unstable crack propagation and arrest in the DCB test specimen. Int J Fracture 1974;10(3):415.
7 Calculation of Energy Release Rate Williams JG. End corrections for orthotropic DCB specimens. Compos Sci Tech 1989;35: Ozdil F, Carlsson LA. Beam analysis of angleply laminate DCB specimens. Compos Sci Technol 1999; 59: Hamed MA, Nosier A, Farrahi GH. Separation of delamination modes in composite beams with symmetric delaminations. J. Materials & Design, 2006;27(10): Herakovich, Carl T. Mechanics of fibrous composites. NewYork: Wiley; Irwin GR, Kies JA. Critical energy release rate analysis of fracture strength. Weld J Res Suppl 1954; 33:193 8.
8
Tensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationFINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND
FINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND COMPARISON WITH EXPERIMENTAL IMPACT TESTS USING NONDESTRUCTIVE VIBROTHERMOGRAPHY EVALUATION A
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationFracture Behavior. Section
Section 6 Fracture Behavior In January 1943 the oneday old Liberty Ship, SS Schenectady, had just completed successful sea trials and returned to harbor in calm cool weather when... "Without warning and
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationFinite element analysis of diagonal tension failure in RC beams
Finite element analysis of diagonal tension failure in RC beams T. Hasegawa Institute of Technology, Shimizu Corporation, Tokyo, Japan ABSTRACT: Finite element analysis of diagonal tension failure in a
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationIntroduction to Fracture
Introduction to Fracture Introduction Design of a component Yielding Strength Deflection Stiffness Buckling critical load Fatigue Stress and Strain based Vibration Resonance Impact High strain rates Fracture
More informationBRIDGED DELAMINATION CRACKS IN CURVED BEAMS AND MIXEDMODE BENDING SPECIMENS
BRDGED DELANATON CRACKS N CURVED BEAS AND XEDODE BENDNG SPECENS Roberta assabò and Brian N. Cox Department of Structural and Geotechnical Engineering, University of Genova, Via ontallegro, 645, Genova,
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationValidity of fracture mechanics concepts applied to wood by finite element calculation
Wood Sci. Technol. 18:5158 (1984) Wood Science and Technology 9 SpringerVerlag 1984 Validity of fracture mechanics concepts applied to wood by finite element calculation P. Triboulot*, Champenoux, P.
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationFinite Element Analysis of Delamination in Woven Composites under QuasiStatic Indentation
Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, 2013 Finite Element Analysis of Delamination in Woven Composites under QuasiStatic Indentation M. C. Song 1, B.V. Sankar 1, G. Subhash 1,
More informationBeam Models. Wenbin Yu Utah State University, Logan, Utah April 13, 2012
Beam Models Wenbin Yu Utah State University, Logan, Utah 8434130 April 13, 01 1 Introduction If a structure has one of its dimensions much larger than the other two, such as slender wings, rotor blades,
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationDegree Thesis Flexural Rigidity (D) in Beams. Author: Zious Karis. Instructor: Rene Herrmann
Degree Thesis Flexural Rigidity (D) in Beams Author: Zious Karis Instructor: Rene Herrmann Degree Thesis Materials Processing Technology 2017 DEGREE THESIS Arcada University of Applied Sciences, Helsinki,
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationOn the calculation of energy release rates for cracked laminates with residual stresses
International Journal of Fracture, 39, 67 93 006) On the calculation of energy release rates for cracked laminates with residual stresses J. A. NAIRN Wood Science and Engineering, Oregon State University,
More informationInitiation de fissure dans les milieux fragiles  Prise en compte des contraintes résiduelles
Initiation de fissure dans les milieux fragiles  Prise en compte des contraintes résiduelles D. Leguillon Institut Jean le Rond d Alembert CNRS/UPMC Paris, France Parvizi, Garrett and Bailey experiments
More informationPlease refer to the usage guidelines at or alternatively contact
Mollon, V., Bonhomme, Jorge, Elmarakbi, Ahmed, Vina, J. and Arguelles, A. (205) Comparison of numerical, empirical and local partition methods in ADCB specimens. International Journal of Automotive Composites,
More informationThe Initiation and Growth of Delaminations Induced by Matrix Microcracks in Laminated Composites
International Journal of Fracture, 57, 1 4 199. The Initiation and Growth of Delaminations Induced by Matri Microcracks in aminated Composites J. A. NAIRN and S. HU Department of Materials Science and
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationTransactions on Engineering Sciences vol 13, 1996 WIT Press, ISSN
Computational debonding analysis of a thermally stressed fiber/matrix composite cylinder F.G. Buchholz," O. Koca* "Institute ofapplied Mechanics, University ofpaderborn, D33098 Paderborn, Germany ^Institute
More informationAPPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS
APPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS L. Zu, S. Koussios and A. Beukers Design and Production of Composite Structures, Faculty of Aerospace Engineering
More informationPoisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics
10.1111/j.14602695.2007.01095.x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department
More informationCracks Jacques Besson
Jacques Besson Centre des Matériaux UMR 7633 Mines ParisTech PSL Research University Institut Mines Télécom Aγνωστ oς Θεoς Outline 1 Some definitions 2 in a linear elastic material 3 in a plastic material
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationMODELING OF CONCRETE MATERIALS AND STRUCTURES. Kaspar Willam. Isotropic Elastic Models: Invariant vs Principal Formulations
MODELING OF CONCRETE MATERIALS AND STRUCTURES Kaspar Willam University of Colorado at Boulder Class Meeting #2: Nonlinear Elastic Models Isotropic Elastic Models: Invariant vs Principal Formulations Elastic
More informationAccurate ModeSeparated Energy Release Rates for Delamination Cracks
Accurate ModeSeparated Energy Release Rates for Delamination Cracks HaeSoo Oh 1 Dept. of Mathematics, University of North Carolina at Charlotte, Charlotte, NC 831 Email: hso@uncc.edu Key Words: Method
More informationUSE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR
USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More information*MAT_PAPER  a new orthotropic elastoplastic model for paper materials
*MAT_PAPER  a new orthotropic elastoplastic model for paper materials Jesper Karlsson, Dynamore Nordic Mikael Schill, Dynamore Nordic Johan Tryding, Tetra Pak *MAT_PAPER (*MAT_274) A new orthotropic elastoplastic
More informationAspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites
Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationDebonding process in composites using BEM
Boundary Elements XXVII 331 Debonding process in composites using BEM P. Prochazka & M. Valek Czech Technical University, Prague, Czech Republic Abstract The paper deals with the debonding fibermatrix
More informationElasticPlastic Fracture Mechanics. Professor S. Suresh
ElasticPlastic Fracture Mechanics Professor S. Suresh Elastic Plastic Fracture Previously, we have analyzed problems in which the plastic zone was small compared to the specimen dimensions (small scale
More informationLAMB WAVE RESPONSE OF FATIGUED COMPOSITE SAMPLES. Reveiw of Progress in Quantitative Nondestructive Evaluation, Vol 13B (1994) pp.
LAMB WAVE RESPONSE OF FATIGUED COMPOSITE SAMPLES Reveiw of Progress in Quantitative Nondestructive Evaluation, Vol 13B (1994) pp. 12611266 INTRODUCTION Michael D. Seale and Barry T. Smith Departments
More informationIntroduction to scaling issues of damage and fracture in wind turbine blades
Introduction to scaling issues of damage and fracture in wind turbine blades Bent F. Sørensen Composites and Materials Mechanics Section Department of Wind Energy Technical University of Denmark Risø Campus,
More informationUniversity of Bristol  Explore Bristol Research. Publisher's PDF, also known as Version of record License (if available): Unspecified
Garza Rodriguez, C., Smith, D., Shterenlikht, A., & Pavier, M. (2015). Advances in the deep hole drilling technique for the residual stress measurement in composite laminates. In Proc 5th Thematic Conf.
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationProgram: Recent Trends
The SNL/MSU/DOE Fatigue Program: Recent Trends John Mandell Montana State University 2012 SNL Blade Workshop May 30  June 1, 2012 Outline Overview of MSU Fatigue Program on Wind Blade Materials: Testing
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationA PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS
1 A PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS An ESIS Protocol Revised June 2007, Nov 2010 D R Moore, J G Williams
More informationDELAMINATION IN MODE I AND II OF CARBON FIBRE COMPOSITE MATERIALS : FIBRE ORIENTATION INFLUENCE
DELAMINATION IN MODE I AND II OF CARBON FIBRE COMPOSITE MATERIALS : FIBRE ORIENTATION INFLUENCE F. LACHAUD 1,2, R. PIQUET 2, L. MICHEL 1 2 LMT, IUT de énie Mécanique, 50, Chemin des Maraîchers, 31077 TOULOUSE
More information2.2 Fracture Mechanics Fundamentals
. Fracture Mechanics Fundamentals Fracture Mechanics is that technology concerned with the modeling of cracking phenomena. Bulk (smooth specimen) properties are not normally useful in design for determining
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More informationFracture mechanics analysis of coating/substrate systems Part I: Analysis of tensile and bending experiments
Engineering Fracture Mechanics ) 4 Author prepared preprint Fracture mechanics analysis of coating/substrate systems Part I: Analysis of tensile and bending experiments SungRyong Kim a, John A. airn
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationBUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.
More informationDynamic mixedmode I/II delamination fracture and energy release rate of unidirectional graphite/epoxy composites
Engineering Fracture Mechanics 7 (5) 53 558 www.elsevier.com/locate/engfracmech Dynamic mixedmode I/II delamination fracture and energy release rate of unidirectional graphite/epoxy composites Sylvanus
More informationMechanical Design in Optical Engineering
OPTI Buckling Buckling and Stability: As we learned in the previous lectures, structures may fail in a variety of ways, depending on the materials, load and support conditions. We had two primary concerns:
More informationCRACK FORMATION AND CRACK PROPAGATION INTO THE COMPRESSION ZONE ON REINFORCED CONCRETE BEAM STRUCTURES
S. Kakay et al. Int. J. Comp. Meth. and Exp. Meas. Vol. 5 No. (017) 116 14 CRACK FORMATION AND CRACK PROPAGATION INTO THE COMPRESSION ZONE ON REINFORCED CONCRETE BEAM STRUCTURES SAMDAR KAKAY DANIEL BÅRDSEN
More informationA simple planestrain solution for functionally graded multilayered isotropic cylinders
Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000000 1 A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The
More information